Tsutomu Ikeda • Yoichi Tomimura • Kengo Magara Shuji Hosoya
Sulfuric acid bleaching of kraft pulp Ih Behavior of lignin and carbohydrate
during sulfuric acid bleaching
Received: September 24, 1998 / Accepted: December 4, 1998 Abstract The purpose of this study was to investigate the behavior of lignin and carbohydrates in kraft pulps during sulfuric acid bleaching. Beech kraft pulp and red pine kraft pulp were bleached with dilute sulfuric acid at p H 1.3 with addition of sodium nitrate and sodium nitrite at 100°C for 1 h. The pulps were then extracted with aqueous sodium hydroxide solution at 70°C for l h. Lignin and carbohy- drates in the acid effluents and the alkali effluents were analyzed. The carbohydrate compositions of unbleached and bleached kraft pulps were also determined. The re- sidual lignin in kraft pulp was degraded to a molecular size similar to that of milled wood lignin during sulfuric acid bleaching without additives, and it was further degraded to a much smaller molecular size during sulfuric acid bleaching with additives. It was found that the amount of carbohy- drate dissolved in the bleach effluents were only about 1% of the dry weight of the kraft pulp under these bleaching conditions. The carbohydrates dissolved during bleaching were mostly of hemicellulose origin.
Key words Sulfuric acid bleaching • Nonchlorine bleach- ing • Residual lignin • Kraft pulp
Environmental problems, including the discharge of organochloro compounds from kraft bleach plants, have
T. Ikeda • S, Hosoya
Institute of Agricultural and Forest Engineering, University of Tsukuba, 1-1-1 Tennoudai, Ibaraki 305-0006, Japan
Y. Tomimura • K. Magara • S. Hosoya ( ~ )
Wood Chemistry Laboratory, Wood Chemistry Division, Forestry and Forest Products Research Institute, PO Box 16, Tsukuba Norin Kenkyu Danchi-nai, Ibaraki 305-8687, Japan
Tel. +81-298-73-3211, ext. 524; Fax +81-298-73-3797 e-mail: firstname.lastname@example.org
Part of this report was presented at the 8th International Symposium on Wood and Pulping Chemistry, Helsinki, July 1995
recently been one of the greatest concerns of the pulp and paper industry. Worldwide pulp manufacturers, accord- ingly, have been shifting the bleaching technologies from elemental chlorine-based ones to these with no chlorine or lower chlorine levels. As a consequence, the amount of elemental chlorine in use for pulp bleaching has been de- creasing rapidly, chlorine dioxide being substituted for el- emental chlorine to a great extent. Moreover, the amount of oxygen-based bleaching chemicals, such as oxygen, perox- ides, and ozone, has been increasing gradually during the past decade.
In our preceding paper (part I of this series), ~ sulfuric acid bleaching of kraft pulp was proposed as one stage of the nonchlorine bleaching processes. Kraft pulp and oxygen predelignified kraft pulp were successfully bleached with dilute sulfuric acid, keeping the pulp viscosity within acceptable levels. The delignification selectivity was appre- ciably improved by the addition of sodium nitrate and sodium nitrite. The principal chemistry involved in this bleaching, as described previously, 1 is acidolytic fragmenta- tion and solubilization of the residual lignin in kraft pulp. Because kraft pulp has been exposed only to alkaline condi- tions, the residual lignin in kraft pulp could have acid-labile bonds such as vinylether-type interunit linkage in lignin or benzylether-type lignin-carbohydrate linkages. In our ear- lier paper, 2 through characterization of the residual lignin, the resistance of the residual lignin in kraft pulp was ex- plained by these lignin-carbohydrate linkages. The stability of the lignin-carbohydrate linkages during kraft cooking was also confirmed by model experiments in another earlier paper. 3 In addition to acidolytic reactions, some oxidative fragmentation reactions can be expected after adding sodium nitrate and sodium nitrite during sulfuric acid treatment.
removal and hexeneuronic acid removal 4,s to the kappa number reduction during sulfuric acid bleaching, including some lignin model experiments, will be subsequently published.
Species used were Japanese beech (Fagus crenata Blume)
and Japanese red pine (Pinus densiflora Sieb. et Zucc.).
Condition were as follows: active alkali 13.5% (beech), 18% (red pine); sulfidity 25%; liquor ratio 41/kg; cooking temperature and time: maximum 170°C, time to maximum 90min, time at maximum 90rain. The kappa number and viscosity of the pulp were determined by a TAPPI standard method.
Kraft pulp(30g) ] H2SO4 NaNO3 "~ a NaNO; ,/
Dialysis stic Extraction
Acid Lignin [
Alkali Effluent Dialysis Alkali Lignin I
Fig. 1. Sample preparation scheme for acid lignin and alkali lignin in sulfuric acid bleaching of kraft pulps. ~Bleaching was done with and without additives separately
Sulfuric acid bleaching
Kraft pulp was placed in a plastic bag (polyvinylidene chlo- ride), and p H 1.3 aqueous sulfuric acid solution was added to make the pulp consistency 10%. Also added were sodium nitrate (4.5% on beech kraft pulp and 8.1% on red pine kraft pulp) and sodium nitrite (0.9% on each pulp). Then the plastic bag was placed in a boiling waterbath and kept for i h. The same bleaching was also carried out separately without sodium nitrate and sodium nitrite. The pulp was then filtered, and the effluents were collected for lignin and carbohydrate analyses.
in filtrates were analyzed by high performance liquid chro- matography (HPLC). HPLC conditions were as follows: column, Shimadzu Shim-pack ISA-07/$2504 (4.0mm × 25cm); column temperature, 65°C; eluents, H3BO7/KOH buffer gradient; flow rate, 0.6ml/min; detector, Shimadzu FLD-1 fluoresence detector. The total sugar contents of the lignin preparations were obtained from the sum of each sugar.
Carbohydrate analysis of the pulp
The kraft pulp treated with sulfuric acid was then washed with water, placed in a plastic bag again, and extracted with aqueous sodium hydroxide solution at 70°C for lh. The alkali charge was 3% and 4% on pulp for beech kraft pulp and red pine kraft pulp, respectively. The pulp consistency was 10%. The extracted kraft pulp was then filtered and washed with water. The caustic extraction liquor was col- lected for lignin and carbohydrate analyses.
A sample preparation scheme is shown in Fig. 1. The efflu- ents obtained from the sulfuric acid treatment and the caus- tic extraction were neutralized to pH 6.0, dialyzed (Spectra/ Por Membrane MWCO:1000), and freeze-dried. Alkali lignins thus prepared were analyzed by gel permeation chromatography (GPC). The analytical conditions for GPC were as follows: apparatus, ISCO UA-5; column, Sephadex LH-20 (1.5 × 30.0cm); eluents, dioxane/water (8:2); detec- tor, UV 280nm. Acid lignins and alkali lignins (Fig. 1) were hydrolyzed with 3 % sulfuric acid solution in an autoclave at 120°C for i h. The solutions were filtered by 1G4 filter, and the Klason lignin content was determined. Carbohydrates
Sulfuric acid (72%, 3ml) was added to kraft pulps before and after bleaching, and the preparation was hydrolyzed at 30°C for lh. The sulfuric acid was then diluted to 3%, and it was heated in an autoclave at 120°C for lh. The hydroly- sate was neutralized to pH 6.0 and then analyzed by HPLC.
Carbohydrate analysis of the bleach effluents
The bleach effluents from the sulfuric acid treatment and the following caustic extraction were neutralized to pH 6.0, and concentrated sulfuric acid was added to make the sulfu- ric acid concentration 3%. This preparation was kept in an autoclave at 120°C for lb. The hydrolysates were neutral- ized to pH 6.0 and subjected to HPLC analysis.
Results and discussion
Sulfuric acid bleaching of kraft pulp
Table 1. Results of sulfuric acid bleaching of kraft pulps
Parameter Beech kraft pulp Red pine kraft pulp
Before bleaching After bleaching Before bleaching After bleaching
Kappa no. 19.8 4.9 (9.2) 23.0 7.9
Viscosity (cP) 47.4 26.9 (27.0) 31.7 21.0
Data in parentheses are results of bleaching without additives
Bleaching conditions (beech): acid treatment (pH 1.3), 100°C, 60min, 4.5% NaNO3, and 0.9% NaNO2 on pulp. Alkali extraction: 70°C, 60rain, 3% NaOH on pulp
Bleaching conditions (red pine): acid treatment (pH 1.3), 100°C, 60min, 8.1% NaNO3, and 0.9% NaNO2 on pulp. Alkali extraction: 70°C, 60rain, 4% NaOH on pulp
loss, the delignification selectivity was better than oxygen- alkali bleaching. Because the objective of this report is to investigate the behavior of lignin and carbohydrate during sulfuric acid bleaching, bleaching conditions were not var- ied. The viscosities of bleached pulps were rather high during these bleaching runs, so the kappa numbers can be further decreased with possible sacrifice of pulp viscosity by applying a lower p H for the acidic treatment. The effect of p H and the amount of additives on kappa number reduction and viscosity loss were reported elsewhereJ
Isolation of lignin in bleach effluents derived from bleaching without additives
Lignin samples from the bleach effluents were prepared according the scheme in Fig. 1. In the case of bleaching without additives, the amount of acid lignin was negligible for both beech kraft pulp and red pine kraft pulp. The yield of alkali lignin from beech kraft pulp was 0.72% (0.22g) on pulp, and the Klason lignin content was 52.1%. The yield of alkali lignin from red pine kraft pulp bleaching was 0.72% (0.22g) on pulp, and the Klason lignin content was 73.6%. These alkali lignins were subjected to ultraviolet (UV), in- frared, (IR), and G P C analysis (described later) and com- pared with alkali lignins derived from the bleaching with additives (NaNO3 and NaNO2).
Isolation and characterization of lignin in bleach effluents derived from bleaching with additives
Lignin samples from the bleach effluents were prepared according to the scheme in Fig. 1. Two lignin samples were prepared from the effluents gained after both beech kraft pulp bleaching and red pine kraft pulp bleaching: One is acid lignin, which was prepared via dialysis of the acid efflu- ent; the other is alkali lignin, prepared via dialysis of the alkali effluent. The yields of lignin preparations are shown in Table 2. Klason lignin content and the sugar composi- tions of lignin preparations are shown in Table 3.
The yields of acid lignins were comparatively low (Table 2) because lignin is scarcely soluble in acidic water unless it is highly oxidized. Furthermore, the Klason lignin content of the acid lignins was less than 10% (Table 3) for both beech kraft pulp and red pine kraft pulp. The total sugars in
Table 2. Yields of alkali lignin and acid lignin by sulfuric acid bleach- ing of kraft pulps
Kraft pulp Alkali lignin (g) Acid Lignin (g)
Beech 0.341 (1.13%) 0.170 (0.57%)
Red pine 0.352 (1.17%) 0.069 (0.23%)
Data in parentheses are the yield based on 30g kraft pulp See Table 1 for bleaching conditions
the hydrolysates of acid lignins were approximately 30% (Table 3). The rest of the samples were considered to be degradation products from lignin. These results indicated that acid lignins were highly oxidized by sodium nitrate and sodium nitrite, and most of these lignin fractions were not detectable as Klason lignin because of their high solubility in acidic water. This is why only the negligible amount of acid lignin was obtained from bleaching without additives as described above.
The sugar compositions of acid lignin fractions showed that most of the sugars were of hemicellulose origin. In the case of red pine, however, the yield of glucose was too high to believe that it came from glucomannan, suggesting that small cellulose fragments were included in this fraction. It should be noted here that the carbohydrate moiety in acid lignin fractions (also in alkali lignin fractions) are not neces- sarily chemically bonded to lignin. Because the lignin frac- tions were obtained through dialysis of the bleach effluents, some carbohydrate oligomers could possibly be included in these fractions, provided that those carbohydrate oligomers were soluble and were retained after dialysis.
The yields of alkali lignins from beech kraft pulp bleach- ing and red pine kraft pulp bleaching were higher than the corresponding yields of acid lignins (Table 2). The Klason lignin content of alkali lignins was also much higher than that in the corresponding acid lignins (Table 3). The results showed that the alkali lignins were less degraded than acid lignins, which is why those fractions were not dissolved in dilute sulfuric acid and were extracted later with aqueous alkali.
Table 3. Sugar compositions, yield of total sugars, and hydrolysis residues of alkali and acid lignins by sulfuric acid bleaching of kraft pulps
Parameter Beech Red pine
Alkali lignin Acid lignin Alkali lignin Acid lignin
Hydrolysis residue (%)" 52.5 7.1 75.1 8.8
Total sugar (%)~ 17.2 31.0 4.9 29.3
Sugar composition (%)
Glc 4.0 8.9 39.7 48.9
Xyl 95.1 71.9 40.9 20.8
Man - 2.0 9.7 6.6
Ara - 0.5 1.2 0.7
Gal 0.9 16.7 8.5 23.0
See Table 1 for bleaching conditions
Glc, glucose; Xyl, xylose; Man, mannose; Ara, arabinose; Gal, galactose ~The yields are based on the lignin preparations
10 20 30
Elution volume (mt)
Fig. 2. Gel permeation chromatography (GPC) of alkali lignin from beech kraft pulp bleaching and beech milled wood lignin (MWL). Broken line, MWL; dotted line, alkali lignin (without additives); solid line, alkali lignin (with additives)
'!'¢ ,N N
Elution v o l u m e (ml)
Fig. 3, GPC of alkali lignin from red pine kraft pulp bleaching and red pine MWL. Broken line, MWL; dotted line, alkali lignin (without addi- tives); solid line, alkali lignin (with additives)
2.0 ', '
I I I I
240 260 280 300 320
Fig. 4. Ultraviolet (UV) spectra of alkali lignin from red pine kraft pulp bleaching and red pine MWL. Broken line, MWL; dotted line, alkali lignin (without additives); solid line, alkali lignin (with additives)
bleaching). W h e n the additives sodium nitrate and sodium nitrite were not applied during sulfuric acid bleaching, the molecular weight distributions of alkali lignins were similar to those of the M W L s for both beech kraft pulp bleaching (Fig. 2) and red pine kraft pulp bleaching (Fig. 3). However, alkali lignins obtained from the bleaching with additives showed quite different molecular weight distribution pat- terns from the M W L region to the much lower-molecular- weight region (Figs. 2, 3), indicating severe degradation of the residual lignin in kraft pulps by sodium nitrate and sodium nitrite.
Table 4. Sugar compositions and total amounts of sugars in bleach effluents from sulfuric acid bleaching of kraft pulps
Sugar Beech (%) Red pine (%)
Alkali effluent Acid effluent Alkali effluent Acid effluent
Glc 3.6 1.5 16.8 5.5
Xyl 94.5 94.6 46.6 10.4
Man - - 6.2 1.7
Ara 0.3 1.6 7.2 74.5
Gal 1.6 2.3 23.2 7.9
Total (g) 0.07 0.13 0.14 0.20
See Table 1 for bleaching conditions Total sugars are based on 30g kraft pulp
! ¢ J
I / \lu
; l!il ~ i i/r,,t~ ,
ij I t ~ , V
I ' 2 1 0 0 ~ 0 I ~ t , , F , ,
3000 1500 I000
Wavenumber (cm "l)
Fig. 5. Infrared spectra of alkali tignin from red pine kraft pulp bleach- ing and red pine MWL. Broken line, MWL; dotted line, alkali lignin (without additives); solid line, alkali lignin (with additives)
Table 5. Changes in sugar composition of kraft pulps during sulfuric acid bleaching
Sugar Before bleaching After bleaching
Beech (%) Red pine (%) Beech (%) Red pine (%)
Glc 74.6 86.3 75.6 85.3
Xyl 24.8 6.3 23.8 7.8
Man 0.4 6.4 0.4 6.9
Ara 0.1 0.6 0.1 -
Gal 0.1 0.4 0.1 -
See Table 1 for bleaching conditions
kraft pulp was extensively degraded to low-molecular- weight fragments by sodium nitrate and sodium nitrite during sulfuric acid bleaching, which contributed to a re- duction of the kappa number. The effect of additives on the kappa number reduction was reported in part I of this series. 1
Alkali lignins also contained a small amount of carbohy- drates but not as much as did the acid lignins (Table 3). Sugar compositions of acid hydrolysates of alkali lignin showed that the sugars were mostly of hemicellulose origin in the case of beech kraft pulp bleaching. Alkali lignin from red pine kraft pulp bleaching, however, seemed to contain some cellulose fragments, as was observed for acid lignin described above.
lignin was extensively degraded by the additives. Without additives, alkali lignin had a UV absorption maximum at somewhat longer wavelength than MWL. This is pro- bably because of the formation of ring conjugated side- chain structures ( C = C or C = O ) during acidolysis. 6 The IR spectrum of alkali lignin obtained from the bleach- ing with additives was quite different from that of M W L or alkali lignin obtained without additives. The presence of a nitro group was indicated by the strong bond at around 1560cm -~. The introduction of nitro groups under similar reaction conditions were reported previously by Ohi and Kishino in the reactions of lignin model compounds with nitrous acid] These results indicated that the lignin in
Dissolution of carbohydrates during sulfuric acid bleaching with additives (NaNO3 and NaNO2)
the arabinose in red pine kraft pulp was dissolved into the acid effluent (Table 4), which could reasonably be ex- plained by the instability of the arabinose side chain on arabinoglucuronoxylan. Based on the carbohydrate analy- ses of kraft pulps and bleach effluents, it can be said that no serious degradation of carbohydrates took place during sul- furic acid bleaching of kraft pulp at p H 1.3.
Residual lignin in kraft pulp is degraded to a molecular size similar to that of M W L during sulfuric acid bleaching (pH 1.3) without additives. In the presence of the additives (so- dium nitrate and sodium nitrite), the molecular size of the degraded lignin is much smaller; thus the additives con- tribute to a further decrease in the kappa n u m b e r of the bleached pulp. E v e n though acidolytic reactions are in- volved in the reaction mechanisms of sulfuric acid bleach- ing, the dissolution of carbohydrates during bleaching is limited (only about 1%). The carbohydrates dissolved dur- ing bleaching are mostly of hemicellulose origin.
1. Ikeda T, Hosoya S, Tomimura Y, Magara K, Takano I (1999) Sulfu- ric acid bleaching of kraft pulp I: Bleaching of hardwood and soft- wood kraft pulps. J Wood Sci 45:233-237
2. Yamasaki T, Hosoya S, Chert CL, Gratzl JS, Chang H-M (1981) Characterization of residual lignin in kraft pulp. In: International symposium on wood and pulping chemistry, Stockholm, June 9-12, vol 2, pp 34-42
3. Taneda H, Nakano J, Hosoya S, Chang H-M (1987) Stability of a- ether type model compounds during chemical pulping processes. J Wood Chem Technol 7:485-498
4. Vuorinen T, Telman A, Fagerstr6m P, Buchert J, Tenkanen M (1996) Selective hydrolysis of hexeneuronic acid groups and its application in ECF and TCF bleaching of kraft pulps. In: Interna- tional pulp bleaching conference, Atlanta, April 14-18, Book 1, pp 43-51
5. Gellerstedt G, Li J (1996) An HPLC method for the quantitative determination of hexeneuronic acid groups in chemical pulps. Carbohydr Res 294:41-51
6. Lundquist K (1964) On the separation of lignin degradation products. Acta Chem Scand 18:1316-1317